#------------------------------------------------------------------------------
#$Date: 2022-02-01 10:52:50 +0200 (Tue, 01 Feb 2022) $
#$Revision: 272371 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/62/1566218.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1566218
loop_
_publ_author_name
'Vladislav V. Gurzhiy'
'Alina R. Izatulina'
'Maria G. Krzhizhanovskaya'
'Mikhail N. Murashko'
'Dar-ya V. Spiridonova'
'Vladimir V. Shilovskikh'
'Sergey V. Krivovichev'
_publ_section_title
;
 Thermal behavior of uranyl selenite minerals derriksite and
 demesmaekerite
;
_journal_name_full               'Journal of GeoSciences'
_journal_page_first              249
_journal_page_last               259
_journal_paper_doi               10.3190/jgeosci.315
_journal_volume                  65
_journal_year                    2020
_chemical_formula_moiety         'Cu5 H10 O30 Pb2 Se6 U2'
_chemical_formula_sum            'Cu5 H10 O30 Pb2 Se6 U2'
_chemical_formula_weight         2171.98
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     dual
_cell_angle_alpha                88.659(3)
_cell_angle_beta                 79.634(5)
_cell_angle_gamma                89.844(5)
_cell_formula_units_Z            1
_cell_length_a                   5.6594(5)
_cell_length_b                   10.0663(4)
_cell_length_c                   11.9792(5)
_cell_measurement_reflns_used    2810
_cell_measurement_temperature    243(2)
_cell_measurement_theta_max      30.1670
_cell_measurement_theta_min      3.6580
_cell_volume                     671.12(7)
_computing_cell_refinement       'CrysAlisPro 1.171.39.44a (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.44a (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.44a (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/3 (Sheldrick, 2015)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      243(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.3829
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
--------------------------------------------------------------------------
  1  ω    -26.00   1.00   1.00   22.50    --  -15.14 -77.00-150.00   27
  2  ω    -40.00  17.00   1.00   22.50    --  -15.14 -77.00 -30.00   57
  3  ω     39.00 102.00   1.00   22.50    --   16.86 178.00  60.00   63
  4  ω     -2.00  93.00   1.00   22.50    --   16.86  38.00-120.00   95
  5  ω    -57.00  41.00   1.00   22.50    --   16.86 -57.00  90.00   98
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at home/near, Atlas'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0780665000
_diffrn_orient_matrix_UB_12      -0.0268903000
_diffrn_orient_matrix_UB_13      -0.0337964000
_diffrn_orient_matrix_UB_21      0.0884331000
_diffrn_orient_matrix_UB_22      0.0111914000
_diffrn_orient_matrix_UB_23      -0.0491297000
_diffrn_orient_matrix_UB_31      0.0480540000
_diffrn_orient_matrix_UB_32      -0.0640510000
_diffrn_orient_matrix_UB_33      0.0071150000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0376
_diffrn_reflns_av_unetI/netI     0.0614
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            5542
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.497
_diffrn_reflns_theta_min         3.459
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'SuperNova (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    36.646
_exptl_absorpt_correction_T_max  0.238
_exptl_absorpt_correction_T_min  0.049
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.44a (Rigaku Oxford Diffraction, 2018)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    5.374
_exptl_crystal_description       prism
_exptl_crystal_F_000             947
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.063
_exptl_crystal_size_min          0.055
_refine_diff_density_max         2.663
_refine_diff_density_min         -2.358
_refine_diff_density_rms         0.397
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.021
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     197
_refine_ls_number_reflns         3070
_refine_ls_number_restraints     4
_refine_ls_restrained_S_all      1.020
_refine_ls_R_factor_all          0.0445
_refine_ls_R_factor_gt           0.0348
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0283P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0718
_refine_ls_wR_factor_ref         0.0772
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                2598
_reflns_number_total             3070
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            Demesmaekerite_SN_-30C_last.cif
_cod_data_source_block           demesmaekerite_sn_-30C
_cod_database_code               1566218
_chemical_oxdiff_formula         'Pb2 Cu5 U2 Se6 O30'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_reflns_odcompleteness_completeness 99.74
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     28.51
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.5 times of:
  All O(H) groups, All O(H,H) groups
2. Restrained distances
 O14-H14
 0.95 with sigma of 0.02
 O13-H13
 0.95 with sigma of 0.02
 O12-H12
 0.95 with sigma of 0.02
 H15A-O5_$3
 2 with sigma of 0.02
3. Uiso/Uaniso restraints and constraints
Uanis(O3) = Uanis(O6)
Uanis(O10) = Uanis(O9)
Uanis(O8) = Uanis(O7)
4.a Rotating group:
 O15(H15A,H15B)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.587
_oxdiff_exptl_absorpt_empirical_full_min 0.525
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 1.26084(7) 0.91653(3) 0.25253(3) 0.00843(10) Uani 1 1 d . . . . .
Pb1 Pb 0.17142(7) 0.31106(3) 0.19433(3) 0.01358(11) Uani 1 1 d . . . . .
Se1 Se 1.28827(19) 0.88887(8) -0.04641(7) 0.0090(2) Uani 1 1 d . . . . .
Se2 Se 1.2254(2) 1.16891(8) 0.48747(8) 0.0141(2) Uani 1 1 d . . . . .
Se3 Se 0.90637(19) 0.62505(8) 0.22121(8) 0.0113(2) Uani 1 1 d . . . . .
Cu1 Cu 1.000000 0.500000 0.500000 0.0101(3) Uani 1 2 d S . P . .
Cu2 Cu 0.7071(2) 0.44314(10) 0.04631(10) 0.0103(3) Uani 1 1 d . . . . .
Cu3 Cu 0.5643(2) 0.42368(10) 0.38496(10) 0.0122(3) Uani 1 1 d . . . . .
O1 O 1.5222(14) 0.8657(6) 0.3047(6) 0.0196(16) Uani 1 1 d . . . . .
O2 O 1.0025(15) 0.9661(6) 0.1961(6) 0.0203(17) Uani 1 1 d . . . . .
O3 O 1.4470(14) 0.8655(6) 0.0623(5) 0.0149(11) Uani 1 1 d . . . . .
O4 O 1.1596(14) 0.7382(5) -0.0579(6) 0.0140(15) Uani 1 1 d . . . . .
O5 O 1.5176(13) 0.8866(6) -0.1625(5) 0.0126(15) Uani 1 1 d . . . . .
O6 O 1.1568(14) 1.1009(6) 0.3693(5) 0.0149(11) Uani 1 1 d . . . . .
O7 O 1.2399(15) 1.3310(6) 0.4421(6) 0.0212(12) Uani 1 1 d . . . . .
O8 O 0.9563(15) 1.1702(6) 0.5742(6) 0.0212(12) Uani 1 1 d . . . . .
O9 O 1.1803(13) 0.6912(6) 0.2223(5) 0.0135(11) Uani 1 1 d . . . . .
O10 O 0.8868(13) 0.5135(6) 0.3321(5) 0.0135(11) Uani 1 1 d . . . . .
O11 O 0.9802(13) 0.5151(5) 0.1142(5) 0.0083(14) Uani 1 1 d . . . . .
O12 O 0.6935(14) 0.4091(6) 0.5252(5) 0.0145(15) Uani 1 1 d D . . . .
H12 H 0.76(2) 0.334(7) 0.558(8) 0.022 Uiso 1 1 d D U . . .
O13 O 0.4697(13) 0.4576(5) 0.2380(5) 0.0111(14) Uani 1 1 d D . . . .
H13 H 0.363(15) 0.528(7) 0.234(9) 0.017 Uiso 1 1 d D U . . .
O14 O 0.4042(13) 0.3836(5) 0.0067(5) 0.0104(14) Uani 1 1 d D . . . .
H14 H 0.41(2) 0.297(4) -0.024(8) 0.016 Uiso 1 1 d D U . . .
O15 O 0.6990(17) 0.2031(7) 0.3417(7) 0.034(2) Uani 1 1 d . . . . .
H15A H 0.680693 0.181326 0.272018 0.051 Uiso 1 1 d DR U . . .
H15B H 0.857293 0.196246 0.337927 0.051 Uiso 1 1 d R U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
3 -13 5 0.0399
3 2 -14 0.0592
-2 13 -7 0.0239
-4 3 13 0.0446
7 -2 9 0.0377
-2 -13 -4 0.0406
-7 -3 -9 0.0219
0 14 1 0.0073
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 U1 O2 178.3(3) . .
O1 U1 O3 91.0(3) . .
O1 U1 O5 89.1(3) . 2_875
O1 U1 O6 98.5(3) . .
O1 U1 O8 85.9(3) . 2_776
O1 U1 O9 89.0(3) . .
O2 U1 O3 87.3(3) . .
O2 U1 O5 90.4(3) . 2_875
O2 U1 O6 82.8(3) . .
O2 U1 O8 95.4(3) . 2_776
O2 U1 O9 90.4(3) . .
O3 U1 O5 70.7(2) . 2_875
O6 U1 O3 140.5(2) . .
O6 U1 O5 71.1(2) . 2_875
O6 U1 O8 74.0(2) . 2_776
O6 U1 O9 145.8(2) . .
O8 U1 O3 145.3(2) 2_776 .
O8 U1 O5 143.6(2) 2_776 2_875
O8 U1 O9 73.3(2) 2_776 .
O9 U1 O3 72.0(2) . .
O9 U1 O5 142.7(2) . 2_875
O5 Pb1 O4 105.87(19) 2_765 2_665
O11 Pb1 O4 63.56(17) 1_455 2_665
O11 Pb1 O5 149.07(19) 1_455 2_765
O13 Pb1 O4 147.01(19) . 2_665
O13 Pb1 O5 91.4(2) . 2_765
O13 Pb1 O11 87.1(2) . 1_455
O13 Pb1 O14 75.3(2) . .
O14 Pb1 O4 79.8(2) . 2_665
O14 Pb1 O5 81.1(2) . 2_765
O14 Pb1 O11 68.6(2) . 1_455
O3 Se1 O5 100.8(3) . .
O4 Se1 O3 104.2(3) . .
O4 Se1 O5 100.3(3) . .
O6 Se2 O7 98.1(3) . .
O8 Se2 O6 101.9(4) . .
O8 Se2 O7 99.5(3) . .
O9 Se3 O10 100.3(3) . .
O9 Se3 O11 99.7(3) . .
O10 Se3 O11 97.5(3) . .
O7 Cu1 O7 180.0 2_776 1_545
O7 Cu1 O10 90.4(3) 2_776 2_766
O7 Cu1 O10 89.6(3) 2_776 .
O7 Cu1 O10 89.6(3) 1_545 2_766
O7 Cu1 O10 90.4(3) 1_545 .
O10 Cu1 O10 180.00(9) . 2_766
O12 Cu1 O7 99.5(3) . 1_545
O12 Cu1 O7 99.5(3) 2_766 2_776
O12 Cu1 O7 80.5(3) 2_766 1_545
O12 Cu1 O7 80.5(3) . 2_776
O12 Cu1 O10 76.3(3) . .
O12 Cu1 O10 103.7(3) 2_766 .
O12 Cu1 O10 76.3(3) 2_766 2_766
O12 Cu1 O10 103.7(3) . 2_766
O12 Cu1 O12 180.0 . 2_766
O4 Cu2 Cu2 134.6(2) 2_765 2_665
O4 Cu2 O11 89.1(3) 2_765 .
O4 Cu2 O11 88.1(2) 2_765 2_765
O11 Cu2 Cu2 99.14(17) 2_765 2_665
O11 Cu2 Cu2 136.29(17) . 2_665
O11 Cu2 O11 75.8(2) . 2_765
O14 Cu2 Cu2 40.49(19) 2_665 2_665
O14 Cu2 Cu2 41.09(17) . 2_665
O14 Cu2 O4 95.1(3) . 2_765
O14 Cu2 O4 165.6(3) 2_665 2_765
O14 Cu2 O11 169.3(3) . .
O14 Cu2 O11 96.7(2) 2_665 .
O14 Cu2 O11 114.1(2) . 2_765
O14 Cu2 O11 80.6(2) 2_665 2_765
O14 Cu2 O14 81.6(3) . 2_665
O7 Cu3 O12 74.5(2) 1_445 2_666
O7 Cu3 O15 83.4(3) 1_445 .
O10 Cu3 O7 178.6(3) . 1_445
O10 Cu3 O12 105.7(2) . 2_666
O10 Cu3 O15 96.3(3) . .
O12 Cu3 O7 98.0(3) . 1_445
O12 Cu3 O10 80.6(3) . .
O12 Cu3 O12 86.8(3) . 2_666
O12 Cu3 O13 171.9(3) . .
O12 Cu3 O15 89.0(3) . .
O12 Cu3 O15 156.6(3) 2_666 .
O13 Cu3 O7 89.7(3) . 1_445
O13 Cu3 O10 91.6(3) . .
O13 Cu3 O12 93.0(3) . 2_666
O13 Cu3 O15 94.4(3) . .
Se1 O3 U1 119.4(4) . .
Se1 O4 Pb1 124.7(3) . 2_665
Se1 O4 Cu2 129.8(4) . 2_765
Cu2 O4 Pb1 99.8(2) 2_765 2_665
U1 O5 Pb1 105.3(3) 2_875 2_765
Se1 O5 U1 125.3(3) . 2_875
Se1 O5 Pb1 121.7(3) . 2_765
Se2 O6 U1 139.8(4) . .
Se2 O7 Cu1 129.9(4) . 1_565
Se2 O7 Cu3 121.3(4) . 1_665
Cu3 O7 Cu1 102.5(3) 1_665 1_565
Se2 O8 U1 143.6(4) . 2_776
Se3 O9 U1 125.8(4) . .
Se3 O10 Cu1 137.8(3) . .
Se3 O10 Cu3 117.0(4) . .
Cu3 O10 Cu1 95.2(3) . .
Se3 O11 Pb1 107.9(3) . 1_655
Se3 O11 Cu2 116.6(4) . .
Se3 O11 Cu2 122.8(3) . 2_765
Cu2 O11 Pb1 105.3(2) . 1_655
Cu2 O11 Pb1 97.2(2) 2_765 1_655
Cu2 O11 Cu2 104.2(2) . 2_765
Cu1 O12 Cu3 101.1(2) . 2_666
Cu1 O12 Cu3 107.7(3) . .
Cu1 O12 H12 92(7) . .
Cu3 O12 Cu3 93.2(3) . 2_666
Cu3 O12 H12 130(6) . .
Cu3 O12 H12 129(7) 2_666 .
Pb1 O13 H13 88(6) . .
Cu3 O13 Pb1 115.0(3) . .
Cu3 O13 H13 117(6) . .
Pb1 O14 H14 94(6) . .
Cu2 O14 Pb1 112.4(3) 2_665 .
Cu2 O14 Pb1 102.2(3) . .
Cu2 O14 Cu2 98.4(3) . 2_665
Cu2 O14 H14 115(7) . .
Cu2 O14 H14 132(6) 2_665 .
Cu3 O15 H15A 111.6 . .
Cu3 O15 H15B 111.2 . .
H15A O15 H15B 102.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
U1 O1 1.776(8) .
U1 O2 1.783(8) .
U1 O3 2.399(6) .
U1 O5 2.468(6) 2_875
U1 O6 2.360(6) .
U1 O8 2.363(7) 2_776
U1 O9 2.364(6) .
Pb1 O4 2.752(7) 2_665
Pb1 O5 2.641(7) 2_765
Pb1 O11 2.565(6) 1_455
Pb1 O13 2.381(6) .
Pb1 O14 2.487(6) .
Se1 O3 1.722(7) .
Se1 O4 1.703(6) .
Se1 O5 1.724(7) .
Se2 O6 1.694(6) .
Se2 O7 1.706(6) .
Se2 O8 1.682(8) .
Se3 O9 1.691(7) .
Se3 O10 1.708(6) .
Se3 O11 1.708(6) .
Cu1 O7 2.218(7) 1_545
Cu1 O7 2.218(7) 2_776
Cu1 O10 2.219(6) 2_766
Cu1 O10 2.219(6) .
Cu1 O12 1.935(7) 2_766
Cu1 O12 1.935(7) .
Cu2 Cu2 2.983(2) 2_665
Cu2 O4 1.985(6) 2_765
Cu2 O11 2.397(6) 2_765
Cu2 O11 2.015(7) .
Cu2 O14 1.982(6) 2_665
Cu2 O14 1.958(7) .
Cu3 O7 2.058(8) 1_445
Cu3 O10 2.029(7) .
Cu3 O12 1.952(7) .
Cu3 O12 2.372(7) 2_666
Cu3 O13 1.952(6) .
Cu3 O15 2.383(8) .
O12 H12 0.94(2) .
O13 H13 0.94(2) .
O14 H14 0.95(2) .
O15 H15A 0.8916 .
O15 H15B 0.8917 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
_geom_hbond_publ_flag
O12 H12 O8 0.94(2) 2.02(4) 2.927(10) 160(10) 1_545 yes
O13 H13 O9 0.94(2) 1.95(3) 2.884(9) 172(10) 1_455 yes
O14 H14 O3 0.95(2) 1.86(6) 2.741(8) 153(10) 2_765 yes
O15 H15A O5 0.89 2.01 2.823(10) 151.7 2_765 yes
O15 H15B O6 0.89 2.03 2.856(12) 152.8 1_545 yes
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
O3 Se1 O4 Pb1 172.6(4) . . . 2_665
O3 Se1 O4 Cu2 -39.6(5) . . . 2_765
O3 Se1 O5 U1 -91.6(4) . . . 2_875
O3 Se1 O5 Pb1 53.1(4) . . . 2_765
O4 Se1 O3 U1 -93.1(4) . . . .
O4 Se1 O5 U1 161.7(4) . . . 2_875
O4 Se1 O5 Pb1 -53.6(4) . . . 2_765
O5 Se1 O3 U1 163.3(3) . . . .
O5 Se1 O4 Pb1 -83.4(4) . . . 2_665
O5 Se1 O4 Cu2 64.4(5) . . . 2_765
O6 Se2 O7 Cu1 111.6(5) . . . 1_565
O6 Se2 O7 Cu3 -101.2(5) . . . 1_665
O6 Se2 O8 U1 116.4(6) . . . 2_776
O7 Se2 O6 U1 137.4(6) . . . .
O7 Se2 O8 U1 -143.1(6) . . . 2_776
O8 Se2 O6 U1 -121.1(6) . . . .
O8 Se2 O7 Cu1 8.0(6) . . . 1_565
O8 Se2 O7 Cu3 155.2(4) . . . 1_665
O9 Se3 O10 Cu1 35.5(6) . . . .
O9 Se3 O10 Cu3 170.8(4) . . . .
O9 Se3 O11 Pb1 78.3(3) . . . 1_655
O9 Se3 O11 Cu2 -33.1(4) . . . 2_765
O9 Se3 O11 Cu2 -163.6(3) . . . .
O10 Se3 O9 U1 -118.4(4) . . . .
O10 Se3 O11 Pb1 -23.6(4) . . . 1_655
O10 Se3 O11 Cu2 94.6(4) . . . .
O10 Se3 O11 Cu2 -135.0(4) . . . 2_765
O11 Se3 O9 U1 142.0(4) . . . .
O11 Se3 O10 Cu1 136.8(6) . . . .
O11 Se3 O10 Cu3 -87.8(4) . . . .
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
2.7488 -12.7968 5.0768 -0.0421 -0.1495 0.9879
2.6772 1.8415 -14.4772 0.2308 0.9686 -0.0923
-2.3407 12.5631 -6.5853 0.0675 0.2571 -0.9640
-3.7935 3.0340 12.8520 -0.2198 -0.9329 -0.2852
7.3134 -2.4873 8.6646 -0.7969 0.1932 0.5724
-2.2948 -13.4171 -4.0183 0.6757 -0.1557 0.7205
-7.2355 -2.7805 -9.0520 0.9455 -0.2263 -0.2340
0.1619 14.1853 1.4952 -0.4446 0.0996 -0.8902
